### Universidade Federal de Minas Gerais

### Instituto de Ciências Exatas

### Departamento de Química

### Egon Campos dos Santos

**Computational simulation of the pyrite/arsenopyrite **

**interface– galvanic effects in chemical reactivity of minerals **

Belo Horizonte, 2019

### Egon Campos dos Santos

**Simulação computacional da interface **

**pirita/arsenopirita- efeitos galvânicos na reatividade **

**química de minerais **

Belo Horizonte, 2019

Tese de doutorado apresentada ao Departamento de Química do Instituto de Ciências Exatas da Universidade Federal de Minas Gerais sob orientação do Prof. Dr. Hélio Anderson Duarte, como requisito parcial para a obtenção do grau de Doutor em Química, Química Inorgânica, Físico-química inorgânica.

### UFMG/ICEx/ DQ. 1349

i

**Acknowledgements **

The Brazilian people.

My parents: Regina M. Campos, Welington F. Santos. My friend Juliana Y. Kadooca.

Professor Hélio Anderson Duarte. Professor Lars Pettersson.

Dr. Joakim Halldin Stenlid.

My co-workers: Alexandre, Aline, Antônio, Catarina, Claudio, Fernando, Gustavo, Guilherme, Jessyca, Juliana, Maicon, Matheus, Maurício, Mirelle, Pâmella, Paulo, Sabrina, Selma, Thales, Walber.

My friends: Djalma B. Reis, Gabriel Libânio, Giancarlo G. Almeida, Henrique Neiva e Lucas Moreira.

ii

**Contents **

**List of Abbreviations ... iv **

**List of Figures ... vii **

**List of Tables ... xiii **

**Resumo ... xvii **

**Abstract ... xix **

**Chapter 1 – Sulfide minerals and galvanic interactions ... 1 **

**Sulfide minerals and acid rock drainage ...1 **

**Galvanic effects on sulfide minerals oxidation ...5 **

**Pyrite/arsenopyrite galvanic pair ...7 **

**Objective ...9 **

**Chapter 2 - Simulation techniques ...11 **

**Density functional theory ... 11 **

**Plane waves ... 15 **

**Pseudopotentials ... 16 **

**The DFT+U method ... 18 **

**Topological analysis of the electron density ... 20 **

**Density-functional tight-binding theory ... 20 **

**CI-NEB calculations ... 23 **

**Final considerations ... 25 **

**Chapter 3 – Pyrite/arsenopyrite interface formation ...26 **

**Introduction ... 26 **

**Computational details ... 27 **

**Pyrite/arsenopyrite coherent interface construction... 30 **

**Structure and electronic properties ... 33 **

**Interface adhesion and stability ... 43 **

**Conclusion ... 46 **

**Chapter 4 – Pyrite/arsenopyrite interface local reactivity ...48 **

**Introduction ... 48 **

**Methodology details and nomenclature of the systems ... 49 **

**I-SLABs construction starting from the I-BULKs ... 51 **

iii

**Pyrite/arsenopyrite I-SLABs cleavage plane energies... 55 **

**Pyrite/arsenopyrite I-SLABS chemical reactivity in the presence of water ... 56 **

**Final observations ... 58 **

**Chapter 5 – Pyrite/Arsenopyrite interface band offset ...60 **

**FeS****2****/FeAsS interface construction ... 60 **

**The commensurability of the phases ... 61 **

**Interface model ... 62 **

**Computational details ... 63 **

**The band offset calculation approach ... 64 **

**Pyrite and arsenopyrite calculation ... 65 **

**Pyrite/arsenopyrite interface band offset... 67 **

**Environmental implications and conclusion ... 68 **

**Chapter 6 – DFTB2 parametrization for Pyrite/Water interface ...71 **

**Liquid water: a contemporary challenge for simulations ... 71 **

**Water parametrization ... 72 **

**Pyrite “Fe-X” pair parametrization ... 74 **

**Results: Bulk water properties ... 74 **

**Results: Pyrite bulk and surface properties... 80 **

**Results: Water adsorption on pyrite (100) surface ... 82 **

**Conclusion ... 83 **

**Chapter 7 – SO****3**** and SO****4**** formation on pyrite (100) surface ...85 **

**Introduction ... 85 **

**Theoretical framework ... 87 **

**Results and discussion ... 89 **

**Final remarks ... 94 **

**Chapter 8 – Final considerations and perspectives ...98 **

**Bibliography ... 104 ****Appendix ... A1 **

iv

**List of Abbreviations **

**List of Abbreviations**

ARD (Acid Rock Drainage)

B (Bond)

BG (Band Gap)

BM (Bulk Modulus)

BO (Band Offset)

CS (Core Shell)

CBM (Conduction Band Minimum)

CI-NEB (Climbing Image- Nudged Elastic Band)

DFT (Density functional theory)

DFTB (Density-Functional Tight-Binding)

DOS (Density of States)

ELF (Electron Localization Function)

FASP (Framework for Automatization of SLAKO Parametrization)

FS (Final State)

GGA (Generalized Gradient Approximation)

HF (Hartree-Fock)

HATR-IR (Horizontal Attenuated Total Reflectance Infrared)

v HRTEM (High Resolution Transmission Electron Microscopy)

I-BULK (Interface Bulk)

I-SLAB (Interface Slab)

IS (Initial State)

KS (Khom and Sham)

LDA (Local Density Approximation)

LP (Lone Pair)

MEP (Minimum Energy Pathway)

NEB (Nudged Elastic Band)

PBE (Perdew-Burke-Ernzerhof)

PDOS (Projected Density of States)

PES (Potential Energy Surface)

PP (Pseudopotential)

RLCAO (Relativistic Linear Combination of Atomic Orbitals)

RMC (Reverse Monte Carlo)

RP (Rest Potential)

SCC (Self-consistent charge)

SCF (Self-Consistent Field)

SLAKO (Slater-Koster)

vi UFF (Universal Force Field)

VBM (Valence Band Maximum)

VSEPR (Valence Shell Electron Pair Repulsion)

XAS (X-ray Absorption Spectroscopy)

XC (Exchange-Correlation)

vii

**List of Figures **

**List of Figures**

**Figure 1- Sulfide minerals and crystallographic structures. ... 2 ****Figure 2- Self-catalytic oxidation of pyrite. The initial process of pyrite dissolutive ****oxidation is shown. ... 4 ****Figure 3- Dissolution rate (mol.m****-2**_{.s}**-1**_{) for single and two phases system. Obtained }**from Ref. [40]. ... 6 ****Figure 4- Scheme showing the oxidation of arsenopyrite in the presence of pyrite. .... 8 ****Figure 5- Illustration showing the SCF procedure for DFT methods. ... 14 ****Figure 6- Construction of the pseudo wave function 𝝓(𝒓) by the pseudopotential ****method. Figure quoted from Reference [95]... 18 ****Figure 7- Minimum energy path illustration and force decomposition in NEB ****calculations. Figure adapted from Ref. [107]. ... 23 ****Figure 8- Pyrite and arsenopyrite calculated band gaps as function of the Hubbard ****(U-J) parameter. Black and red dashed lines represent the experimental band gap for ****pyrite[166, 167] (0.90 eV) and arsenopyrite[119, 168] (0.82 eV), respectively. ... 28 ****Figure 9- Scheme showing how to construct a coherent interface model that increases ****the overlapping area, 𝑺𝑨/𝑩, between phase A and B. ... 31 ****Figure 10- Interface structure. In (a) is shown the interface layered structure along ****the c-axis. In (b) are shown the pyrite and arsenopyrite bulk, where is highlighted the ****two Fe-Fe bond distances (short and long) in the structure of arsenopyrite. In (c) are ****shown the interfacial Fe-Fe bonds and the interface types. From left to right the ****interfaces in (c) are: FeS****2****(100)/FeAsS(001), FeS****2****(100)/FeAsS(100)-As, and ****FeS****2****(100)/FeAsS(100)-S. The red, yellow, and green spheres represent, respectively, ****the Fe, S, and As atoms. The red dotted lines represent the normal interfacial plane ****formed by the contact of the two phases. ... 36 **

viii
**Figure 11- Strain influence in the electronic structure of pyrite (a) and arsenopyrite ****(b) minerals. ... 37 ****Figure 12- Electron localization function (ELF) for (a) FeS****2****(100)/FeAsS(001), (b) ****FeS****2****(100)/FeAsS(100)-As, and (c) FeS****2****(100)/FeAsS(100)-S interface planes located in ****the pyrite region (left side) and arsenopyrite region (right side). The axial Fe-X bonds ****are shown in Figure A6. ... 38 ****Figure 13- (Left) Illustration of the structure of arsenopyrite and (Right) isosurface ****and section of the 4c-2e electron state at -2.5 eV below Fermi level, calculated at the **** point. The Isosurface factor of 0.01 e/Å****3**_{ was set. Color code: yellow - Sulfur, green - }**Arsenic, brown -Iron. ... 40 ****Figure 14- Density of states (DOS) projected for the interface atoms in the range of -8 ****to 4 eV: (a) is the FeS****2****(100)/FeAsS(001) system, (b) the FeS****2****(100)/FeAsS(100)-S, and ****(c) the FeS****2****(100)/FeAsS(100)-As system. The band gap (BG) was calculated from the ****band structures shown in Figure A7. ... 41 ****Figure 15- Projected density of states. “Bulk” and “Int” meanings the density of states ****from the bulk region and interface region, respectively. ... 42 ****Figure 16- Nomenclature used in the present Chapter for (a) pyrite and arsenopyrite ****crystal bulk, (b) pyrite and arsenopyrite surface, (c) interface bulk (I-BULKs). ... 50 ****Figure 17- I-SLABs obtained from the I-BULKs. The blue dot lines represent the ****cleavage plane perpendicular [(1)**_{⊥}**] to the interface, and the red dot lines the four ****parallel cleavage planes close to the interface region [(1)****ǁ**** ,(2)****ǁ**** ,(3)****ǁ**** , and (4)****ǁ****]. The ****red, yellow and green spheres represent the iron, sulfur and arsenic atoms in the ****structures above. The doted circles show the iron sites that were used to adsorb water ****molecules. ... 52 ****Figure 18- Structure and Charge density difference, 𝜟𝝆, for the interfaces. (a) is the ****FeS****2****(100)/FeAsS(001) interface, (b) the FeS****2****(100)/FeAsS(100)-As interface, and (c) ****the FeS****2****(100)/FeAsS(100)-S interface. Isosurfaces are shown for 0.01 e/Å****3****. Red, ****yellow, and green spheres represent, respectively, the Fe, S, and As atoms. ... 54 **

ix
**Figure 19- Water adsorption on the “FeS****2****(100)/FeAsS(100)-As” I-SLABs. (a) ****adsorption on the parallel I-SLAB model, (b) adsorption on the perpendicular I-SLAB ****with the water located in the pyrite side, and (c) water adsorption on the ****perpendicular I-SLAB with the water located in the pyrite side. ... 57 ****Figure 20- Interface model construction. (a) is the FeS****2****(100) pyrite bulk, (b) the ****FeAsS(100)-As arsenopyrite bulk, and (c) the FeS****2****(100)/FeAsS(100)-As interface. The ****FeS****2****(100)/FeAsS(001) and FeS****2****(100)/FeAsS(100)-As constructions are shown in ****Figure A12 and Figure 16, respectively. ... 61 ****Figure 21- Displacement calculation for the FeS****2****(100)/FeAsS(100)-As interface ****model. The results found for the FeS****2****(100)/FeAsS(001) and FeS****2****(100)/FeAsS(100)-S ****interfaces are shown, respectively, in Figure A10 and Figure A11. ... 65 ****Figure 22- Valence band maximum (VBM) and Conduction band minimum (CBM) vs ****(U-J) Hubbard parameter for (a) pyrite and (b) arsenopyrite bulk minerals. Vertical ****lines represents the band gaps obtained for (U-J)= 1.5 eV. Grey shaded regions mean ****the occupied states level. ... 66 ****Figure 23- Interface frontier’s orbitals for the FeS****2****(100)/FeAsS(100)-As interface. ****The results found for the FeS****2****(100)/FeAsS(001) and FeS****2****(100)/FeAsS(100)-S ****interfaces are shown, one-to-one, in Figure A13 and Figure A15. ... 67 ****Figure 24- Interface band offset for (a) FeS****2****(100)/FeAsS(001), (b) ****FeS****2****(100)/FeAsS(100)-As, and (c) FeS****2****(100)/FeAsS(100)-As interfaces. Grey shaded ****areas mean the occupied states level. The upper panel shows qualitatively the band ****alignment obtained for the three FeS****2****/FeAsS interfaces. ... 68 ****Figure 25- O-O and O-H radial distribution function obtained at different ****temperatures for neutral water. Experimental values quoted from Refs. [235-237].*** ... 75 *
**Figure 26- Water-matsci, water-matsci-UFF, matsci and the experimental (FREE, Ref. ****[236]) distribution of the angles O****1****-Oc-O****1****. All calculations were done for liquid water ****at 298 K. ... 76 **

x
**Figure 27- Pyrite projected density of states in the vicinity of Fermi level. Inset figure ****represents pyrite unit cell. ... 81 ****Figure 28- Water adsorption on pyrite (100) surface. Color code: yellow, sulfur; ****brown, iron; red, oxygen; and white, hydrogen. ... 83 ****Figure 29- Pyrite oxidation mechanism in aqueous medium explained by Type I and ****Type II reactions. Figure quoted from Ref. [185]. ... 86 ****Figure 30- Side (a) and top (b) view of pyrite slab used in all calculations. Fragment ****of pyrite (c) used to show the reactions. Colour code: yellow - Sulfur, brown - Iron. . 88 ****Figure 31- Fragment of pyrite (100) surface depicting the initial steps of pyrite ****oxidation. Energies in electronvolt and bond distances in Angstrom. Colour code: ****yellow - Sulfur, red – oxygen, white – hydrogen, brown - Iron. ... 90 ****Figure 32- SO****2**** dissociation on pyrite surface to form (SO****2****)****d****. ... 91 ****Figure 33- (SO****3****)****d****, (HSO****3****)****d****, (HSO****4****)****d**** and (SO****4****)****d**** formation on pyrite surface by Type II ****reactions. ... 92 ****Figure 34- (SO****4****)****d**** and (HSO****4****)****d**** and formation on pyrite surface by Type III reactions.**

* ... 93 *
**Figure 35- (SO****3****)****d**** and (HSO****3****)****d**** and formation on pyrite surface by Type III reactions.**

* ... 93 *
**Figure 36- Scheme showing the oxidation mechanism of pyrite (100) surface in three ****different stages [(1), (2) and (3)]. Activation energies (E****a****) for stage (1) quoted from ****literature.[185] All “E****a****“ calculations are in the same theoretical level. Values in ****electronvolt [eV]. ... 96 ****Figure 37- Scheme showing how complex is the oxidation of pyrite/arsenopyrite ****interface in ambient conditions. ... 102 ****Figure A1- Convergence test for the total energy as a function of the K-points meshes. ****In the graph E****1x1x1**** represents the total energy for the calculation at the Γ point and **

xi
**n****atom**** is the total number of atoms in the pyrite unit cell. In all calculations, the cutoff ****of 80 Ry was used. ... A1 ****Figure A2- Convergence test for the total energy as a function of the cutoff. In the ****graph E****30**** represents the total energy for the calculation with 30 Ry cutoff and n****atom**** is ****the total number of atoms in the pyrite unit cell. In all calculations, the 6x6x6 K-points ****meshes was used. ... A1 ****Figure A3- Convergence test for the total energy as a function of the K-points meshes. ****In the graph E****1x1x1**** represents the total energy for the calculation at the Γ point and ****n****atom**** is the total number of atoms in the pyrite unit cell. In all calculations, the cutoff ****of 80 Ry was used. ... A2 ****Figure A4- Convergence test for the total energy as a function of the cutoff. In the ****graph E****30**** represents the total energy for the calculation with 30 Ry cutoff and n****atom**** is ****the total number of atoms in the pyrite unit cell. In all calculations, the 6x6x6 K-points ****meshes was used. ... A2 ****Figure A5- Crystallographic transformation of the arsenopyrite (010) surface from ****triclinic to an orthorhombic structure... A5 ****Figure A6- Electron localization function for (a) FeS****2****(100)/FeAsS(001), (b) ****FeS****2****(100)/FeAsS(100)-As, and (c) FeS****2****(100)/FeAsS(100)-S Fe-X****ax**** bonds. ...A11 ****Figure A7- Band structure. BG meanings the band gap of the interfaces. K-Path ****G-Y-H-C-E-M1-A-Z-D-G-A-X-H1-G from the monoclinic lattice. ...A12 ****Figure A8- Structures used to calculate the formation energy of the interfaces and the ****pyrite and arsenopyrite bulk. ...A13 ****Figure A9- Interface cleavage planes along the (010) direction. (a), (b) and (c) ****represents, one-to-one, the interfaces: FeS****2****(100)/FeAsS(001), FeS****2****(100)/FeAsS(100)-As, and FeS****2****(100)/FeAsS(100)-S. The blue line is the plane direction, and dashed ****ellipses indicate the cleaved As-S and S-S bonds. ...A14 **

xii
**Figure A10- Displacement calculation for the FeS****2****(100)/FeAsS(001) interface model.**

* ...A16 *
**Figure A11- Displacement calculation for the FeS****2****(100)/FeAsS(100)-S interface ****model. ...A16 ****Figure A12- Illustration showing the FeS****2****(100)/FeAsS(001) interface model ****construction from pyrite and arsenopyrite isolated phases. ...A17 ****Figure A13- (left) VBM and (right) CBM states for the FeS****2****(100)/FeAsS(001) interface ****model. ...A17 ****Figure A14- Illustration showing the FeS****2****(100)/FeAsS(100)-S interface model ****construction from pyrite and arsenopyrite isolated phases. ...A18 ****Figure A15- (left) VBM and (right) CBM states for the FeS****2****(100)/FeAsS(100)-S ****interface model. ...A18 ****Figure A16- Radial distribution function for O-O obtained by RMC NVT molecular ****dynamics. It includes the original matsci RDF. ...A19 ****Figure A17- Radial distribution function for O-O obtained by RMC NVT molecular ****dynamics. It includes the original matsci RDF. ...A19 ****Figure A18- Radial distribution function for O-O obtained by RMC. NVT and NVE ****molecular dynamics. ...A20 ****Figure A19- Radial distribution function for O-H obtained by RMC. NVT and NVE ****molecular dynamics. ...A20 ****Figure A20- DFT and DFTB2 band structure of iron-FCC (a) and pyrite (b) bulk ****structures. ...A21 ****Figure A21- SO dissociation on pyrite surface. Color code: yellow - Sulfur, green - ****Arsenic, brown -Iron. ...A23 **

xiii

**List of Tables **

**List of Tables**

**Table 1- Rest potential for different sulphide minerals at pH 4. Values quoted from ****Ref. [25]. ... 5 ****Table 2: Formation energy, E****f****, for pyrite and arsenopyrite phases. |Δ| represents the ****percentage error between the calculated value and the experimental value. ... 29 ****Table 3: Pyrite and arsenopyrite mismatch parameter, 𝜉, calculation. All the 𝜉 values ****were calculated considering the (100) surface of pyrite. In brackets are the surface ****energy values for the surfaces related to the most stable interfaces estimated by our ****theoretical level. ... 32 ****Table 4: Work of adhesion, W****ad****, and formation energy for the most stable interfaces. ****W****pyrite**** and W****arsenopyrite**** meanings the work of self-adhesion for pyrite and arsenopyrite, ****respectively. ... 45 ****Table 5- Surface energy calculated for the different cleavage planes shown in Figure ****17. ... 56 ****Table 6- Values of 𝒒 parameter in the distribution of 𝜽𝑶𝑶𝑶angles for different DFTB2 ****parameter sets compared to values from RMC fits to scattering data of Ref. [236]. . 78 ****Table 7- Neutral water self-diffusion coefficient (Å****2**_{/ps) of the oxygen atom at }**different temperatures. Quoted references in parenthesis. ... 79 ****Table 8- Water adsorption energy (calculated by Eq. (4.3)) and Fe-OH**_{2}**distance. DFT ****values quoted from Ref. [185]. ... 82 ****Table A1: Pyrite Hubbart (GGA+U) parameter test. The cutoff of 50 Ry and the K-point ****of 4x4x4 were used in all the calculation. BG meanings the band gap of the system for ****the tested GGA+U parameters. ... A3 ****Table A2: Arsenopyrite Hubbart (GGA+U) parameter test for arsenopyrite structure. ****The cutoff of 50 Ry and the K-point of 4x4x4 were used in all the calculation. ... A4 **

xiv
**Table A3: Arsenopyrite Hubbart (GGA+U) parameter test for arsenopyrite structure ****and band gap (BG). The cutoff of 50 Ry and the K-point of 4x4x4 were used in all the ****calculations. ... A4 ****Table A4: Fe-X****eq**** and X-S bond distances of the three interfaces. ... A6 ****Table A5- Fe-X****ax**** and interfacial contact distances, δ**_{0}**, of the three interface systems. ****In the red parenthesis are the percentage difference** between the interfaces ****structure parameters and the arsenopyrite bulk structure. In the green brackets are ****the percentage difference** between the interfaces and the arsenopyrite bulk. ... A6 ****Table A6: Spin test for the arsenopyrite (001) surface. “TM” meanings the total ****magnetization of the system and “AM” the absolute magnetization of the system. The ****cutoff of 50 Ry and the K-point of 4x4x4 were used in all the calculations. ... A7 ****Table A7: Spin test for the arsenopyrite (100)-As surface. “TM” meanings the total ****magnetization of the system and “AM” the absolute magnetization of the system. The ****cutoff of 50 Ry and the K-point of 4x4x4 were used in all the calculations. ... A7 ****Table A8: Spin test for the arsenopyrite (100)-S surface. “TM” meanings the total ****magnetization of the system and “AM” the absolute magnetization of the system. The ****cutoff of 50 Ry and the K-point of 4x4x4 were used in all the calculations. ... A7 ****Table A9: Py(100)/AsPy(001) total energy. The cutoff of 50 Ry and the K-point of ****4x4x4 were used. In all the calculations the lattice parameters were fixed, and only ****the atom positions were allowed to move freely in the optimization process. ****Highlighted in red the structure with the lowest energy. ... A8 ****Table A10: FeS****2****(100)/FeAsS(100)-As total energy. The cutoff of 50 Ry and the K-point ****of 4x4x4 were used. In all calculations the lattice parameters were fixed, and only the ****atom positions were allowed to move freely in the optimization process. Highlighted ****in red the structure with the lowest energy. ... A8 ****Table A11: FeS****2****(100)/FeAsS(100)-S total energy. The cutoff of 50 Ry and the K-point ****of 4x4x4 were used. In all calculations the lattice parameters were fixed, and only the **

xv
**atom positions were allowed to move freely in the optimization process. Highlighted ****in red the structure with the lowest energy. ... A8 ****Table A12: Spin teste for the FeS****2****(100)/FeAsS(001) interface. “ALT” meanings that ****alternated initial spin states were used, following the sequencie Up-Down-Up-Down ****for the iron, sulfur and arsenic sites in the interface region. “Up” meanings all spin ****states up and “O” that no spin polarization was used for the atoms in the DFT SCF ****calculations. “TM” is the total magnetization, and “AM” the absolute magnetization. ****The cutoff of 50 Ry and the K-point of 4x4x4 were used. ... A9 ****Table A13: Spin teste for the FeS****2****(100)/FeAsS(100)-As interface. “ALT” meanings that ****alternated initial spin states were used, following the sequencie Up-Down-Up-Down ****for the iron, sulfur and arsenic sites in the interface region. “Up” meanings all spin ****states up and “O” that no spin polarization was used for the atoms in the DFT SCF ****calculations. “TM” is the total magnetization, and “AM” the absolute magnetization. ****The cutoff of 50 Ry and the K-point of 4x4x4 were used. ...A10 ****Table A14: Spin teste for the FeS****2****(100)/FeAsS(100)-S interface. “ALT” meanings that ****alternated initial spin states were used, following the sequencie Up-Down-Up-Down ****for the iron, sulfur and arsenic sites in the interface region. “Up” meanings all spin ****states up and “O” that no spin polarization was used for the atoms in the DFT SCF ****calculations. “TM” is the total magnetization, and “AM” the absolute magnetization. ****The cutoff of 50 Ry and the K-point of 4x4x4 were used. ...A10 ****Table A15: Structural parameters obtained for the structures shown in Figure A8.*** ...A13 *
**Table A16: Hubbard parameter (U-J) test for pyrite isolated mineral. A cutoff of 40 Ry ****and 6x6x4 k-point mesh were used in all the calculations. BG means the band gap of ****the system for the tested (U-J) parameters. ...A15 ****Table A17- Hubbard parameter (U-J) test for arsenopyrite structure. A cutoff of 40 Ry ****and 6x6x4 k-point mesh were used in all the calculations. BG means the band gap of ****the system for the tested (U-J) parameters. (%𝒆𝒓𝒓𝒐 **) ...A15 **

xvi
**Table A18- (U-J) influencie in band offset calculation. All the calculation were done ****following the Eq. (1). For the total energy calculation it was used the 4x4x2 k-points ****grid and the cutoff of 40 Ry. ...A15 ****Table A19- Repulsion energy parametrization. Atomic pairs, reference systems, ****dependencies for a-b pairs, E****bnd**** and E****ref**** interception point (IP), the cut radius (R****cut****), ****and bond distances. Only singlet spin configuration was considered for all reference ****systems. ...A22 **

xvii

**Resumo **

**Resumo**

Efeitos galvânicos desempenham um papel importante no mecanismo de oxidação de sulfetos minerais. A pirita (FeS2) é o sulfeto mineral mais abundante na Terra e, na

presença de arsenopirita (FeAsS), sua oxidação diminui. Consequentemente, a taxa de oxidação de arsenopirita é aumentada, liberando as espécies As(III) e As(V) no meio. Estas espécies são um perigo para o meio ambiente e podem se tornar um problema de saúde nas regiões de mineração. Nesta tese reportamos a investigação do par galvânico gerado pela interface pirita/arsenopirita a partir de cálculos DFT/ondas planas (Capítulo 3). Para construir os modelos de interface, inicialmente testou-se a comensurabilidade entre a superfície (100) de pirita (superfície de pirita com maior ocorrência na natureza) com as doze superfícies de arsenopirita relatadas na literatura. Dentre todas as superfícies avaliadas, foram construídas as interfaces mais estáveis e avaliadas a sua estabilidade junto com suas propriedades eletrônicas. Como a pirita e arsenopirita apresentam diferentes (i) distâncias de ligação e (ii) parâmetros das redes cristalinas, não é possível combinar perfeitamente as fases. Como consequência, sítios octaédricos distorcidos e tensões estruturais são formados na região interfacial. Esta observação está de acordo com a análise do trabalho de adesão estimado e com os cálculos de energia de formação. Ambos os parâmetros sugerem que a formação da interface pirita/arsenopirita não é termodinamicamente favorável. Isto está de acordo com o que é observado em amostras naturais.

A reatividade local das interfaces foi avaliada a partir da adsorção de água (Capítulo 4). Foram encontrados valores de adsorção comparáveis entre as três interfaces FeS2/FeAsS

e as fases isoladas (FeS2 e FeAsS). Isto sugere que a possível formação da interface ocorre

sem modificar as propriedades ácido-base de Lewis dos sítios ativos na ruptura do
*material. Cálculos de Band Offset (Capítulo 5) mostraram que seus valores de band gap *
das interfaces são pelo menos três vezes menores que os valores encontrados para a pirita
ou a arsenopirita isoladas. Uma vez que os sulfetos minerais são materiais
*semicondutores que podem participar de reações eletroquímicas, a diminuição do band *
*gap facilita a transferência de elétrons ao longo de sua estrutura. Este fato contribui para *
explicar por que as interações galvânicas aumentam a oxidação de arsenopirita na
presença de pirita. O presente estudo ressalta a importância de efeitos galvânicos para
entender o mecanismo de oxidação da arsenopirita na presença de pirita.

xviii Foi desenvolvida uma metodologia capaz de simular a interface água/pirita (capítulo 6). É sabido na literatura que o método DFTB2 não descreve bem propriedades estáticas e dinâmicas da água líquida. Por isso foi feito a reparametrização dos parâmetros DFTB2 a partir de uma correção empírica da energia de repulsão DFTB2 construindo os parâmetros nomeados nesta tese como water-matsci. Funções radiais do tipo O-O e O-H foram descritas com ótimo acordo com dados experimentais. Além disso, os novos parâmetros são capazes de descrever a tetraedralidade das moléculas de água nas temperaturas de 298 e 254 K. Finalmente, foi observado que a modificação dos parâmetros não modifica a energia de adsorção de água na superfície (100) da pirita.

Os cálculos de uma nova rota para a oxidação da espécie adsorvida SO2 amplia a

compreensão do mecanismo de oxidação da pirita (Capítulo 7). Até o momento apenas as etapas iniciais do processo de oxidação da pirita foram feitas a partir de cálculos teóricos. De acordo com os nossos cálculos, observa-se que a dissociação da espécie SO2 pode

ocorrer sobre a superfície (100) da pirita. A energia de ativação (0.44 eV) foi estimada em aproximadamente metade do valor da energia de ativação da etapa limitante da reação global (0.80 eV), o que sugere que esta espécie pode ser formada na superfície da pirita. Além do mais, a espécie SO2 leva a formação dos intermediários SO3 e SO4 com energias

de ativação menores que 0.16 eV (valor 5 vezes menor que a etapa limitante). Outro aspecto importante do mecanismo proposto por nossos cálculos é o fato que a molécula de oxigênio é capaz de reagir com a espécie SO2 na superfície. Esse tipo de reação sobre a

superfície da pirita ainda não tinha sido explorado por cálculos teóricos, porém já tinha sido sugerido com análises experimentais. A rota investigada de oxidação do SO2

adsorvido pelo oxigênio molecular foi denominada reações do Tipo III que ocorrem na superfície da pirita.

**Palavras-chave: Sulfetos minerais, pirita, arsenopirita, pares galvânicos, interfaces, DFT, **
DFTB.

xix

**Abstract **

**Abstract**

Galvanic effects play an important role in the oxidation mechanism of sulfide minerals. Pyrite (FeS2) is the most common sulfide mineral in the Earth, and in the presence of

arsenopyrite (FeAsS) its oxidation is delayed and the oxidation rate of arsenopyrite is increased, releasing As(III) and As(V) species in the medium. These arsenic ions are an environment hazards and become health problem in the vicinities of the mining regions. We report a DFT/plane waves study of the pyrite/arsenopyrite galvanic cell (Chapter 3). To build the interface models we tested the commensurability of the pyrite (100) surface (the pyrite surface with highest occurrence in the nature) with the twelve arsenopyrite surfaces reported in the literature. Among all evaluated surfaces the most stable interfaces were built, and their structure, stability, and electronic properties were evaluated. As pyrite and arsenopyrite have different (i) bond distances and (ii) crystal lattice parameters, it is not possible to perfectly match the phases, and distorted octahedral sites are formed in the interfacial region. Consequently, strained structures are observed. This structural observation agrees with the word of adhesion and the formation energy analysis. Both parameters suggest that the formation of FeS2/FeAsS interface is

not favourable. This is in agreement with what is observed in natural samples.

The local reactivity of the interfaces was evaluated by water adsorption energies (Chapter 4). Comparable adsorption values were found among the interfaces (FeS2/FeAsS) and

isolated phases (FeS2 and FeAsS). This suggests that the possible interface formation

would occur without modifying the Lewis acid-base properties of the active sites in the event of material rupture. Band offset (Chapter 5) calculations for the most stable interfaces showed that their band gap values are at least three times lower than the values found for the pure pyrite or arsenopyrite. Since sulfide minerals are semiconductor materials that can participate in electrochemical reactions, the decrease in the band gap thus facilitates electron transfer at the pyrite/arsenopyrite interface. This fact contributes to explain why the galvanic interactions increase the oxidation of arsenopyrite in the presence of pyrite. The present study underlines the importance of galvanic effects to understand the oxidation mechanism of arsenopyrite in the presence of pyrite.

It was developed a methodology capable of simulating the water/pyrite interface (chapter 6). It is known in the literature that the DFTB2 method does not describe well static and

xx dynamic properties of liquid water. Therefore, the DFTB2 parameters were reparametrized from an empirical correction of the DFTB2 repulsion energy by constructing the parameters labelled in this thesis as water-matsci. Radial functions of type gO-O and gO-H were described in agreement with experimental data. In addition, the new parameters are capable of describing the tetrahedrality of the water molecules at temperatures 298 and 254 K. Finally, it was observed that the modification of the parameters does not modify the water adsorption energy at the pyrite surface (100).

All calculations of a new route for the adsorbed SO2 oxidation extend the knowlegment

about the pyrite oxidation mechanism (Chapter 7) As far as we know, only the initial stages of the pyrite oxidation process have been made from theoretical calculations. According to our calculations, it is observed that the dissociation of SO2 species can occurs

on the surface. The activation energy (0.44 eV) was estimated to be approximately two times the activation energy of the limiting step of the global reaction (0.80 eV), suggesting that this species can be formed on the pyrite surface. Moreover, the SO2 species leads to

the formation of adsorbed SO3 and SO4 species on the surface with activation energies

lower than 0.16 eV (this value is 5 times less than the rate limiting step). Another important aspect of the mechanics proposed by our calculations is the fact that oxygen molecule is capable to react with the SO2 species on the surface as it was suggested by

experimental analyses, but up to date, it was not theoretically calculated. The investigated route for the adsorbed SO2 oxidation by the molecular oxygen was labelled as Type III

reactions that occur on the pyrite surface.

**Key-words: Sulfide Minerals, pyrite, arsenopyrite, galvanic couples, interfaces, DFT, **
DFTB.

1

**Chapter 1 – Sulfide minerals and galvanic interactions **

**Chapter 1 – Sulfide minerals and galvanic interactions**

**Preamble: Noble and base metals of economic importance are normally associated to **
metal sulfides (pyrites) and their extraction may imply in important environmental
impact, mostly due to the acid rock drainage (ARD). When exposed to atmosphere and
humidity, sulfide minerals are oxidized to form sulfuric acid in the medium. In addition,
the oxidation of mineral sulfides directly affects soil quality, since toxic metals and
metalloids (such as Hg, As and Cd) are released in the environment. Several factors act
accelerating oxidation processes of these minerals, and the association of two or more
minerals in galvanic pairs greatly aggravates the rate of dissolution of these minerals. This
work aims to study the galvanic interaction between pyrite and arsenopyrite. Pyrite is the
most abundant sulfide mineral and it is mostly responsible for the formation of ARD
products. Arsenopyrite is also associated with gold, copper ores, among others, and in
nature and its dissolution process releases arsenic into the environment.

**Sulfide minerals and acid rock drainage**

**Sulfide minerals and acid rock drainage**

Sulfide minerals are considered the most diverse minerals in terms of its physical,
chemical, and structural properties (Figure 1). Such diversity originates from their more
complex crystal and electronic structures when compared to other class of materials.[1,
2] The main reasons are found in the variety of oxidation states, coordination numbers,
symmetry, density and stoichiometry. Furthermore, sulfide minerals can participate in
both acid–base and redox reactions, thus their exposed surfaces can be the place where
*different reaction mechanisms can occur. Accordingly to Vaughan et al.,[3] the electrical *
and magnetic properties of metal sulfides are arguably the most diverse found in any
group of materials. They are diamagnetic insulators (e.g. ZnS), diamagnetic
semiconductors (e.g. FeS2, PbS, and FeAsS), antiferromagnetic semiconductors (e.g.

CuFeS2), and even magnetic and non-magnetic metallic conductors (e.g. Fe7S8 and Fe9S10).

Recently, new developments have been achieved in superconductor synthesis, such as CuS.[4, 5] On this sense, several new technological materials are synthesized exploring the properties of these minerals. Their applications are broad: production of solar and photochemical cells, solid batteries, superconductors and in heterogeneous catalysis.[6]

2 Another important point is the fact that it has been argued that sulfide minerals can catalyze reactions responsible for the origin of life on Earth.[7, 8]

**Figure 1- Sulfide minerals and crystallographic structures. **

Sulfide minerals form one of the most important classes of minerals and are source of non-ferrous metals on Earth, hence different processes of metal extraction are used in the mining industry.[9] There are two possible routes for obtaining the metals from the sulfide minerals. Traditionally, the preferred route is the pyrometallurgical. Although widely used, the pyrometallurgical process is currently less attractive due to the lower copper content in the available ore in nature, increasing the extracting cost of the desired metals. An alternative to the pyrometallurgical extraction procedure, is the hydrometallurgical process. The latter process is based on ore leaching, which consist in extracting an element component through their dissolution in a solution. The advantage of the hydrometallurgical route is that it is able to treat ores with low metal content, making it more economically viable than the pyrometallurgical route.

Besides the industrial/economic importance of the sulfide minerals, they have been studied due to the consequences of their spontaneous oxidative dissolution when they are exposed to the environment.[10, 11] The technological and environmental importance of this phenomenon makes it an important subject of research from both fundamental and industrial perspectives. Particularly, sulfide minerals when exposed to atmospheric air and humidity are oxidized to form sulfuric acid in the medium. This

3
phenomenon is called Acid Rock Drainagei_{ (ARD) and has several consequences for the }

balance of biological and chemical systems found in the environment.[9] The ARD solutions carry significant environmental problems because ARD waters can be harmful to humans and other life forms.[10, 12] A major problem related to ARD is the acidification of aquifers near mining areas. This directly disturbs all the biodiversity around the affected areas. In addition, the oxidation of mineral sulfides directly affects soil quality, since toxic metals (such as Hg, As and Cd) are released to the environment.

The ARD chemical reactions can be explained considering the pyrite oxidative process. It is the most abundant sulfide mineral and a reference for studying other important mineral sulfides.[13] The pyrite oxidation reactions are given in Eqs. (1.1)– (1.5). The initial step is described in Eq. (1.1), where the dissolution of the mineral occurs, forming the SO42-, Fe2+, and H+ ions in the medium. After the oxygen molecule reacts with

pyrite releasing Fe2+_{(aq), acid and sulfates, the Fe}2+_{(aq) ions are subsequently oxidized to }

Fe3+_{ (Eq. (1.2)). As the concentration of Fe}3+_{ increases, the oxidation proceeds following }

the reaction described by Eq. (1.3) increasing the pH of the medium. As the concentration
of dissolved Fe3+_{ decreases with increasing pH, parallel Fe}3+_{ precipitation reactions occur }

forming hydroxides (Fe(OH)3) and oxy-hydroxides (FeOOH), following the Eq. (1.4) and

Eq. (1.5), respectively.

FeS2 + 7/2O2 + H2O = Fe2+ + 2SO42- + 2H+ **(1.1) **

Fe2+ _{+ 1/4O}_{2 }_{+ H}+_{ = Fe}3+ _{+1/2 H}_{2}_{O } _{(1.2) }

FeS2 + 14Fe3+ + 8H2O = 15Fe2+ + 2SO42- + 16H+ **(1.3) **

Fe3+ _{+ 3H}_{2}_{O = Fe(OH)}_{3 }_{+ 3H}+ _{(1.4) }

Fe3+ _{+ 2H}_{2}_{O = FeOOH + 3H}+ _{(1.5) }

Comparing the oxidation reactions of the different mineral sulfides, it is possible to comprehend the general reactions of the process as a self-catalytic cycle. Taking again pyrite as a reference, Figure 2 shows a simple scheme that summarizes the oxidative process of sulfide minerals. Initially, the oxidation occurs by the O2 and H2O agents. In

aqueous media or even in direct contact with the air, both molecules are present, and can oxidize any sulfide mineral. The former reaction release ions in the medium (in the case

4
of pyrite, it releases ferric ion in the medium). The ferric ions (Fe(III)) act as oxidant
agents of the pyrite surface forming ferrous (Fe(II)) ions. The ferrous ions react with the
oxygen molecule and the hydronium to form again the ferric ion. A Fe2+_{/Fe}3+_{ cycle }

between the iron species occurs until the oxidation reaction finishes.

Numerous factors can affect the oxidation kinetics of the mineral sulfides. Generally, sulfides dissolution oxidation are accelerated (or retarded) by several factors including pH,[14] oxidant type (eg. O2 and Fe3+),[15-17] oxidant concentration,[15-17]

grain size,[18, 19] and non-sulfide minerals (the most common is the SiO2). Oxidation is

further complex since the electrochemical nature of sulfides are affected by trace element
contents such as Cu, Zn, Ni, Co, Ag, As, Ti, Mg, Mn, Al and Si. Then, the exact chemical
composition of the sample will dictate the specific oxidation pathway.[20-24] ARD is a
spontaneous process, nevertheless its production is also catalyzed in the presence of the
*bacterial species: Acidithiobacillus ferrooxidans, Acidithiobacillus thiooxidans and *
*Leptospirillum ferrooxidans. Different reaction pathways are also observed in the *
presence of these microorganisms.

**Figure 2- Self-catalytic oxidation of pyrite. The initial process of pyrite dissolutive ****oxidation is shown.**

Chemical, biological and physical factors added to intrinsic characteristics of each mine make ARD highly variable site-to-site. Furthermore, there are no standardized methods for measure or reducing the risk of ARD in the environment.[10] Likewise, the separation of sulfide minerals (generally pyrite from the other minerals) by flotation and leaching methods increases the costs for mining industry.[10, 18] It has been reported

5 [18] that the cost to treat and remediate ARD mining concentrates in the word are more than 100 billion dollars. New approaches for predicting and mitigating the ARD can only be envisaged if its mechanism is understood in detail at a molecular level.

**Galvanic effects on sulfide minerals oxidation **

**Galvanic effects on sulfide minerals oxidation**

In addition to the factors mentioned above, it is extremely important to consider that sulfide minerals are associated forming galvanic pairs. In nature, sulfurous ores are complex solid mixtures and, consequently, their structural, mechanical and especially their electrochemical properties are difficult to be assessed. Nowadays, hydrometallurgical routes are also considered for treating low-grade ores instead of pyrometallurgical processes. However, the secondary reactions provoked by the galvanic interactions between associated minerals within the concentrates can prevent the recovery of noble metals. In aqueous leaching or bioleaching systems the galvanic interaction substantially increases the oxidative dissolution of one or both of the minerals that constitute the galvanic cell.[25-39] This will depend on the electrochemical characteristics of the minerals and on the occurrence of the distinct sulfides contained in the soils, sediments, substrates and ore concentrates. Since pyrite is ubiquitous mineral in Earth’s, it is commonly found associated with other important minerals, such as: sphalerite,[40] galena,[25, 26, 37] marcasite,[25] covellite,[25, 40] bornite,[25, 40] chalcopyrite[40-47] and arsenopyrite.[48-55]

**Table 1- Rest potential for different sulphide minerals at pH 4. Values quoted from ****Ref. [25]. **

Mineral Formula unit RP,*V vs. SHE *

Pyrite FeS2 0.66 Marcasite FeS2 0.63 Chalcopyrite CuFeS2 0.56 Spharelite ZnS 0.46 Covelite CuS 0.45 Bornite Cu5FeS4 0.42 Galena PbS 0.40 Argenite Ag2S 0.28 Stibnite Sb2S3 0.12 Molybdenite MoS2 0.11

6 The contact of distinct sulfide minerals initiates the galvanic effect in the presence of an electrolyte. One mineral will act as anode promoting the oxidation reaction and the other as cathode, in which the reduction reaction occurs.[29, 56] The reactivity of minerals forming mixtures or solid solutions can be measured from its rest potential (RP), see Table 1.[25, 29, 30, 36, 38] As previously defined,[25] the RP of a mineral electrode is the potential difference across the mineral–solution interface when the mineral surface is at electrical equilibrium with respect to electrochemical processes. Pyrite has the highest RP among the sulfides, thus, pyrite is the least reactive sulfide minerals, and, consequently, it will rule the oxidation process of the other associated minerals.[25, 33] Consequently, pyrite acts as a cathode in the oxidative process and more reactive sulfides as an anode (see Table 1).

**Figure 3- Dissolution rate (mol.m****-2**_{.s}**-1**_{) for single and two phases system. Obtained }**from Ref. [40]. **

One might argue that the ideal formula is not found naturally for any mineral, and trace element contents are responsible to vary the absolute value of pyrite RP. Notwithstanding, electrochemical measurements for a large number of samples from a

7 variety of geological environments showed a slight variation in the rest potentials measurements.[30, 38, 57] The data suggest that the rest potentials are more affected by the galvanic processes due to the associated minerals than by its elemental composition. Therefore the galvanic processes are the most important effect governing the dissolution rate of sulfide minerals in hydrometallurgical and natural systems.[57]

Abraitis et al.[40] studied the kinetics of metal sulfides oxidation in acidic medium
(pH 2.5 and 25 °C) monitoring the cation products (Zn2+_{, Fe}2+_{, Cu}+_{ and Pb}2+_{) by ICP-AES }

(Inductively Coupled Plasma- Atomic Emission Spectroscopy). In order to compare the oxidative behaviour of the target minerals and measure the influence of the galvanic effects in the reaction, the author studied at the same conditions the oxidation of the isolated phases and their oxidation in the presence of pyrite. The studied systems were galena/pyrite, chalcopyrite/pyrite, sphalerite/pyrite, pyrite, galena, and chalcopyrite. The oxidation rates obtained after 200 min of reaction are shown in Figure 3. The results showed that in the presence of pyrite the dissolution of sulfides mixed-mineral systems can be dramatically affected by galvanic effects, and the rates can increase by factor as greater than 3 or 5 times if compared with the isolated phases in the same experimental conditions. By analysing in detail the results shown in Figure 3, it is possible to observe that the galena/pyrite galvanic pair presented an anomalous result, being the dissolution rate of the interface around 30 times greater than the oxidation of the isolated phases.

**Pyrite/arsenopyrite galvanic pair **

**Pyrite/arsenopyrite galvanic pair**

In the study of the galvanic interactions between sulfide minerals, a better understanding of the pyrite/arsenopyrite galvanic interaction is important by many reasons. Arsenopyrite (FeAsS) is an important mineral because it is primarily associated with other sulfide minerals and valuable metals (e.g., copper, silver, and gold). In certain ores, it has considerable economic significance since it carries the major portion of gold in the ore. Its exposition to the environment leads to acid rock drainage releasing arsenite [As(III)] and arsenate [As(V)] in addition to acid and heavy metals, which is hazardous for the environment. Also, arsenopyrite environmental problems have been a major concern in the mineral industry.

8
Natural arsenopyrite samples are always associated with pyrite, and in its
composition generally it is found large randomly contact domains of pyrite distributed in
its structure.[58-61] In several studies the galvanic pair formed by arsenopyrite and
*pyrite minerals increases the dissolution oxidation process.[48-55] Urbano et al.[55] *
carried out a voltammetric study of arsenopyrite containing 11.84% of pyrite
mineralogical impurity and compared the results to the oxidation of a natural pyrite
mineral containing 98.96% of purity. The authors concluded that the reactivity in the
presence of galvanic effects are electrochemically modified, and the pyrite oxidation is
delayed when it is associated to the arsenopyrite. Consequently, the oxidation process of
arsenopyrite is enhanced with larger production of arsenic in the medium.

* Figure 4- Scheme showing the oxidation of arsenopyrite in the presence of pyrite. *
The electrochemical behaviour of pyrite and arsenopyrite minerals in contact to
each other has been intensely investigated.[30, 54] It has been found that oxidation of the
pyrite/arsenopyrite is similar to the isolated pyrite or arsenopyrite, and a large quantity
of sulfate is produced. However, the reaction mechanism has not been identified. Other
authors[25, 48, 53, 55] found that pyrite oxidation proceeds via a complex sequence of
series and parallel reaction steps which can be proposed from the electrochemical data.
Briefly, the oxidation of arsenopyrite in the presence of pyrite can be understood
according to the scheme shown in Figure 4, where a sequence of cathodic and anodic
reactions is shown.

9

**Objective**

**Objective**

The knowledge about the surface chemistry of these minerals and their chemical reactivity is the first step to understand and determine the oxidation mechanism of the mineral sulfides. Its relevance is related to the development of improved methods for controlling the ARD and for metal extraction with better environmental performance are present. Many studies on the reactivity of mineral sulfides are available in the literature.[45, 48, 55] The reactivity of the minerals is directly related to their atomic structure, composition, geometry and its electronic properties. Computer simulation of this intricate reactions can provide insights about the reaction mechanism at a molecular level and help to interpret the large experimental data reported in the literature. The development of efficient computational methods makes computational chemistry an important tool for investigating the microscopic behaviour of these mineral surfaces. Density Functional Theory (DFT) is widely used for investigating reactions and is particularly important in the study of solid phase materials. The DFT enables accurate estimates of the chemical properties in a reasonable calculation time. Recently, modelling the oxidation mechanism of pyrite[62, 63] and arsenopyrite[64] in the presence of oxygen and water has been subject of investigations. However, to the best of our knowledge, no tentative to model the pyrite inlay in arsenopyrite has been modelled.

The main objective of this thesis is to provide initial insights on structural and electronic properties of the pyrite/arsenopyrite interface and its comparison with the results for the isolated pyrite and arsenopyrite are provided. To achieve this goal, the following steps were pursued:

1. To study the crystalline phases of pure pyrite and arsenopyrite minerals, and then
**identify their most favoured surfaces exposed in nature (chapter 3). **

**2. To propose a model of the pyrite associated with arsenopyrite (Chapter 3). **
3. To study the stability and the electronic structure of the pyrite/arsenopyrite

interface and compare to the electronic structure of the isolated phases of pyrite
**and arsenopyrite (Chapter 3). **

4. To evaluate the local reactivity of slabs based on the interface-bulk structures
**obtained in chapter 3 (Chapter 4). **

10 5. To study the galvanic interaction of pyrite/arsenopyrite by means of the Band

**Offset (Chapter 5). **

In parallel, two other topics were studied in this thesis.ii

6. To develop DFTB (more details in Chapter 2) parameters in order to describe
**liquid water in contact with pyrite (100) surface (Chapter 6). **

7. To extend our understanding of the oxidation mechanism of pyrite to include the
**formation of S-containing species (Chapter 7). **

11

**Chapter 2 - Simulation techniques **

**Chapter 2 - Simulation techniques**

**Preamble: Density functional theory (and its approximation DFTB) has been used with **
remarkable success in many fields and it is the first-choice method for investigating the
solid state. The simulation codes can calculate a vast range of structural, electronic,
chemical, and thermodynamic properties. In this Chapter, we present an overview of the
fundaments of DFT and its applications. Not all the theoretical aspects will be approached
in this work, additional discussions can be found in the quoted references.

**Density functional theory **

**Density functional theory**

The development of quantum mechanics in the early twentieth century made feasible the estimation of structural, electronic, electrical, and mechanical properties of solids and molecules. Although the analytical solution of the Schrödinger equation is limited to systems containing only one electron, approximate numerical methodologies allow the solution of a multielectron problem with an acceptable level of accuracy. Among these methodologies, the Hartree-Fock (HF) method stands out, although the electronic correlation is neglected. The correlation energy is important to describe many chemical processes, and can be included in the calculations by the so-called post-Hartree-Fock[65-68] (such as: Møller–Plesset perturbation, coupled-cluster, and configuration interaction) methods, and alternatively, by the Density Functional Theory (DFT). When compared to post-Hartree-Fock methods, the DFT method has lower computational cost, and because of that in the last decades DFT has been widely used to describe the electronic structure of large systems containing hundreds of atoms. Particularly, the DFT approach has been broadly used in the study of solids, surfaces, and interfaces. Therefore, in this work the DFT was chosen as a base methodology to perform the computations.

The practice of using the electronic density, 𝜌(𝒓), as a basic variable was first performed by Drude[69, 70] in early twentieth century. According to Drude,[71] the electron behaviour in a metal can be described as an homogenous gas and apply the kinetic theory of gas. Such approximation permitted to describe the thermal and electric conduction properties providing numbers with the same order of magnitude as the

12 experimental values. Starting from Drude’s ideas different models have been developed,[71, 72] however, the use of 𝜌(𝒓) as a basic variable was only validated as an exact theory with the publication of two theorems by Hohenberg and Kohn (HK) in 1964.[73] These two theorems provided the fundamentals of the modern DFT. The HK theorems proves that the ground state of an electron system is a functional of the electron density, and in principle with the knowledge of the electron density only it is possible to calculate all the properties of the system. The first theorem of HK states that the external potential, 𝜈(𝒓), is a unique functional of the electronic density. In other words, it shows that the electron density of a system determines the external potential, 𝜈(𝒓) and the number of electrons, N:

𝑁 = ∫ 𝜌(𝒓)𝑑𝒓. **(2.1) **

The Hamiltonian, 𝐻̂, of the system is given by:

𝐻̂ = 𝑇̂+ 𝑉̂𝑒+ 𝑈̂. **(2.2) **

In Eq. (2.2) 𝑇̂ is the kinetic energy operator, 𝑉̂𝑒 is the repulsion operator related to the

electron-electron classical and non-classical interactions. 𝑈̂ is the electron-core operator
defined by the atomic nucleus charge, 𝑍_{𝐴}, atomic position, 𝑹_{𝛼}, and electron position, 𝒓_{𝒊}:

𝑈̂ = ∑ ∑ − 𝑍𝛼
|𝑹_{𝛼}− 𝒓_{𝒊}|
𝑀
𝐴
𝑁
𝑖
= ∑ 𝜈(𝒓_{𝒊})
𝑁
𝑖
. **(2.3) **

The second HK theorem establishes the DFT variational principle. Since the exact
electronic density describing the system is not known, an approximate electron density
𝜌̃(𝒓) will provide an energy equal to or greater than the exact energy of the system,
(𝐸[𝜌̃] ≥ 𝐸[𝜌] = 𝐸_{0}).

In 1965, Khom and Sham[74] developed a methodology that allows the DFT
calculations as it is done currently. Accordingly to Levy,[75] the Kohn-Sham equations can
be interpreted as the solution of a non-interacting electron system that lead to the
electron density of the interacting system. The Hamiltonian has an effective local
potential, 𝜈_{𝑒𝑓𝑓}(𝒓) , which generates the electron density of the interacting electron
system:

13 𝐻𝐾𝑆 = −1

2𝛻𝑖

2_{+ 𝜈}

𝑒𝑓𝑓(𝒓). **(2.4) **

To obtain the fundamental state of this reference system, 𝛹𝐾𝑆_{, the wave function }

is approximated by an antisymmetric-product of N Kohn-Sham orbitals of an electron,
𝜓_{𝑖}𝐾𝑆(𝒓_{𝒊}), represented by Slater's determinant:

𝛹𝐾𝑆_{= } 1
√𝑁!||
𝜓_{1}𝐾𝑆(𝒓_{𝟏}) 𝜓_{2}𝐾𝑆(𝒓_{𝟏}) … 𝜓_{𝑁}𝐾𝑆(𝒓𝟏)
𝜓_{1}𝐾𝑆(𝒓_{𝟐}) 𝜓_{2}𝐾𝑆(𝒓_{𝟐}) … 𝜓_{𝑁}𝐾𝑆(𝒓𝟐)
⋮
𝜓_{1}𝐾𝑆(𝒓_{𝑵})
⋮
𝜓_{2}𝐾𝑆(𝒓_{𝑵})
⋱ ⋮
… 𝜓_{𝑁}𝐾𝑆(𝒓_{𝑵})
||. **(2.5) **

The one electron Kohn-Sham orbitals, 𝜓_{𝑖}𝐾𝑆_{, and their eigenvalues, 𝜀}

𝑖, are obtained

from the Schrödinger-like equation:

(−1 2𝛻

2_{+ 𝜈}

𝑒𝑓𝑓) 𝜓𝑖𝐾𝑆(𝒓𝒊) = 𝜀𝑖𝜓𝑖𝐾𝑆(𝒓𝒊), **(2.6) **

and the electron density of the reference system can be calculated as a function of 𝜓_{𝑖}𝐾𝑆_{(𝒓}
𝒊)
by the Eq. (2.7).
ρ(𝐫) = ∑ 𝑛_{𝑖}|𝜓_{𝑖}𝐾𝑆(𝒓_{𝒊})|2
𝑁
𝑖
, **(2.7) **

The effective potential is local potential that is defined according to the following equation:

𝜈_{𝑒𝑓𝑓}(𝒓) = 𝜈(𝒓) + ∫ 𝜌(𝒓𝟏)

|𝒓 − 𝒓_{𝟏}|𝑑𝒓𝟏+ 𝜈𝑥𝑐(𝒓), **(2.8) **

where the second term on the right side represents the Coulomb potential, and 𝜈_{𝑥𝑐}(𝒓) is
the potential due to the exchange-correlation energy, 𝐸𝑥𝑐[𝜌]. The former potential can be

defined as the functional derivative of 𝐸_{𝑥𝑐}[𝜌] with respect to 𝜌(𝒓), as indicated in the Eq.
**(2.9). **

𝜈𝑥𝑐(𝒓) =

𝛿𝐸_{𝑥𝑐}[𝜌]

14
Briefly, the KS method consists of using a reference system in which the electrons
do not interact, but which has the same electron density of the real system. This reference
system is solved through the Schrödinger equation, Eq. (2.6), which includes a local
effective potential. The solution of this equation follows the protocol to solve the equation
of the Hartree-Fock method, and the wave function must be expressed by a Slater
determinant, Eq. (2.5). Since the effective potential, 𝜈_{𝑒𝑓𝑓}(𝑟), depends on the electronic
density, 𝜌(𝑟), the KS equations are solved by means of the Self-Consistent Field (SCF)
procedure, Figure 5.

**Figure 5- Illustration showing the SCF procedure for DFT methods. **

Finally, the KS scheme allows to calculate the total electronic energy of the ground
state:
𝐸_{0}[ρ(𝐫)] = ∑ 𝜀_{𝑖}
𝑁
𝑖
−1
2∫
ρ(𝐫)ρ(𝐫′)
|𝒓 − 𝒓′_{|} 𝑑𝒓𝑑𝒓′+ 𝐸𝑥𝑐− ∫ ρ(𝐫)𝜈𝑥𝑐(𝒓)𝑑𝒓. **(2.10) **

Since the exact analytical form of the 𝜈_{𝑥𝑐} potential is not known, Eq. (2.9), these XC
functionals are constructed from different approximations. Several works have been
devoted to the development and test of the different approximations of the
Exchange-correlation functional.[76-78] Basically, three approaches are mostly used for DFT
quantum calculations: Local Density Approximation (LDA, references [79, 80]),

15 Generalized Gradient Approximation (GGA, references [81-86]) and hybrid functional[65, 87-92] are some of the most used XC functionals.

**Plane waves **

**Plane waves**

The inherent symmetry features of the solids is normally used to decrease the
computer efforts and the number of atoms explicitly treated in the structure.[6] From a
microscopic point of view, a crystalline solid can be represented as a minimum set of
lattice points in a periodically-repeating environment, termed unit cell.[72] Since the
macroscopic solid is defined by the translation of the unit cell, we can define a translation
**vector R in real space. The Hamiltonian that describes the electrons in a crystalline solid **
is divided into the kinetic energy of the electrons, and the potential energy that obeys the
following property: 𝑉(𝒓 + 𝑹) = 𝑉(𝒓) . This is periodic boundary condition that is
reinforced to assure the periodicity of the crystalline solid. Bloch's theorem[71, 72] states
that the eigenvectors can be written in the form of a plane wave (𝑒𝑖𝑲.𝒓_{) multiplied by the }

periodic function 𝑢_{𝑛,𝒌}(𝒓), as established in:

𝜓𝑛,𝒌(𝒓 + 𝑹) = 𝜓𝑛,𝒌(𝒓) = 𝑒𝑖𝑲.𝒓 𝑢𝑛,𝒌(𝒓), **(2.11) **

**here K are vectors in reciprocal space and 𝑢**_{𝑛,𝒌}(𝒓) Bloch orbitals have the following
property: 𝑢_{𝑛,𝒌}(𝒓) = 𝑢_{𝑛,𝒌}(𝒓 + 𝑹), consequently 𝜓_{𝑛,𝒌}(𝒓 + 𝑹) = 𝜓_{𝑛,𝒌}(𝒓). The term “n” in Eq.
**(2.11), is known as the band index,[71] and for each K-point the Schrödinger equation is **
solved to obtain a set of eigenvectors and eigenvalues. The set of “n” eigenvalues for the
**different K-points is known as the band structure. **

To solve Schrödinger’s equations, it is convenient to expand the wave function into a set of basis functions. For these systems, the 𝑢𝑛,𝑘(𝒓) is expanded into plane wave basis

sets (∑ 𝐶𝑮 𝑖,𝑮𝑒𝑖𝑮.𝑟**), where G is a vector in the reciprocal space (i.e. a G-vector is the **

**representation of a R-vector in the Brillouin zone). Hence, the Eq. (2.11) is written as: **

𝜓𝑛,𝒌(𝒓) = ∑ 𝐶𝑖,𝒌+𝑮𝑒𝑖(𝒌+𝑮).𝒓, 𝐺

16
This expansion is normally truncated based on a kinetic energy cutoff (calculated by the
expression: (−1 2⁄ )|𝒌 + 𝑮|2_{)). }

Substituting the Eq. (2.12) in the Kohn-Sham expression, Eq. (2.6), we arrive at the
following expression:
(−1
2𝛻
2_{+ 𝜈}
𝑒𝑓) ∑ 𝐶𝑖,𝒌+𝑮𝑒𝑖(𝒌+𝑮).𝒓
𝐺
= 𝜀𝑖∑ 𝐶𝑖,𝒌+𝑮𝑒𝑖(𝒌+𝑮).𝒓
𝐺
. **(2.13) **

By multiplying Eq. (2.13) by 𝑒−𝑖(𝒌+𝑮′).𝒓_{ and integrating over the coordinate space, 𝒓, we }

arrive at a particular form of the Kohn-Sham equation,[93] as shown in Eq. (2.14),

∑ [1
2|𝒌 + 𝑮|
2_{𝛿}
𝑮𝑮′+ 𝑉𝑖𝑜𝑛(𝑮 − 𝑮′) + 𝑉𝐻(𝑮 − 𝑮′) + 𝑉𝑥𝑐(𝑮 − 𝑮′)]
𝐺
= 𝜀𝑖𝐶𝑖,𝒌+𝑮, **(2.14) **

where the first term on the left is the kinetic energy, being 𝛿_{𝑮𝑮′} represented by the
following integral:

𝛿𝑮𝑮′ = ∫ 𝑒𝑖(𝑮−𝑮′).𝒓𝑑𝒓. **(2.15) **

The electron-core attraction, 𝑉𝑖𝑜𝑛(𝑮 − 𝑮′) , coulombian electron-electron repulsion,

𝑉_{𝐻}(𝑮 − 𝑮′_{), and the exchange/correlation, 𝑉}

𝑥𝑐(𝑮 − 𝑮′), potentials are defined in terms of

their Fourier transform, as indicated in Eq. (2.16).

𝑉𝑮−𝑮′= ∫ 𝑉(𝒓) 𝑒𝑖(𝑮−𝑮′).𝒓𝑑𝒓 **(2.16) **

The resolution of Eq. (2.14) is done by diagonalizing the 𝐻_{𝐾+𝐺,𝐾+𝐺} Hamiltonian matrix,
which elements are given on bracketed terms of Eq. (2.14).

**Pseudopotentials **

**Pseudopotentials**

Expanding the wave function of a periodic system in a set of plane waves is a challenge by two main reasons. First, because heavy atoms have a very large number of electrons to be treated, which requires many plane waves to describe the electronic